Protein patterning by microcontact printing using ... Protein patterning by microcontact printing...
Embed Size (px)
Transcript of Protein patterning by microcontact printing using ... Protein patterning by microcontact printing...
Protein patterning by microcontact printing using pyramidal PDMS stamps
Luisa Filipponi1 & Peter Livingston1 & Ondřej Kašpar2 & Viola Tokárová2 & Dan V. Nicolau1,2
Published online: 19 January 2016 # The Author(s) 2016. This article is published with open access at Springerlink.com
Abstract Micro-contact printing, μCP, is a well-established soft-lithography technique for printing biomolecules. μCP uses stamps made of Poly(dimethylsiloxane), PDMS, made by replicating a microstructured silicon master fabricated by semiconductor manufacturing processes. One of the problems of the μCP is the difficult control of the printing process, which, because of the high compressibility of PDMS, is very sensitive to minute changes in the applied pressure. This over- sensitive response leads to frequent and/or uncontrollable col- lapse of the stamps with high aspect ratios, thus decreasing the printing accuracy and reproducibility. Here we present a straightforward methodology of designing and fabricating PDMS structures with an architecture which uses the collapse of the stamp to reduce, rather than enlarge the variability of the printing. The PDMS stamp, organized as an array of pyrami- dal micro-posts, whose ceiling collapses when pressed on a flat surface, replicates the structure of the silicon master fab- ricated by anisotropic wet etching. Upon application of pres- sure, depending on the size of, and the pitch between, the PDMS pyramids, an air gap is formed surrounding either the entire array, or individual posts. The printing technology,
which also exhibits a remarkably low background noise for fluorescence detection, may find applications when the clear demarcation of the shapes of protein patterns and the distance between them are critical, such as microarrays and studies of cell patterning.
Keywords Poly(dimethylsiloxane) microstructures . Protein patterning .Microcontact printing . Soft-lithography . Protein microarrays
Patterning proteins on surfaces have multiple applications in the area of biomedical microdevices, such as microarrays (Allison et al. 2006; Müller and Nicolau 2005), lab-on-a- chip (Chin et al. 2012), biosensors and bioMEMS (Mujahid et al. 2013), as well in the area of functional studies for cell and tissue development (Kane et al. 1999; Nicolau et al. 1996; Nicolau et al. 1999a). The patterning of proteins can be achieved by their immobilisation from solution in contact with surfaces presenting pre-fabricated patterns, using either selec- tive covalent binding (Ivanova et al. 2002; Lenci et al. 2011; Nicolau et al. 1998, 1999b), or more rarely selective adsorp- tion (Lan et al. 2005; Nicolau et al. 1999b). This strategy, which typically uses photolithographic techniques (Fodor et al. 1991), and even standard resist materials (Ivanova et al. 2002; Nicolau et al. 1998, 1999b), has the inherent ad- vantage of high resolution of printing, at the expense of high cost of ownership and possible low signal/noise ratio due to the non-specific binding from protein solutions on areas out- side the pattern of interest. Alternatively, protein patterns can be created by direct deposition methods, such as projection- based printing, e.g., ink-jet printing (Pardo et al. 2003), or based on laser microablation (Dobroiu et al. 2010), or
Electronic supplementary material The online version of this article (doi:10.1007/s10544-016-0036-4) contains supplementary material, which is available to authorized users.
* Dan V. Nicolau firstname.lastname@example.org
1 Industrial Research Institute Swinburne, Faculty of Engineering and Industrial Science, Swinburne University of Technology, PO Box 218, VIC 3122, Australia
2 Faculty of Engineering, Department of Bioengineering, McGill University, Macdonald Engineering Building, Room 378, 817 Sherbrooke Street West, Montreal, QC H3A 0C3, Canada
Biomed Microdevices (2016) 18: 9 DOI 10.1007/s10544-016-0036-4
contact-based printing, e.g., classical pin printing (Rowland et al. 2012), dip pen lithography (Huo et al. 2008), or microcontact printing, μCP (Bernard et al. 1998; Kumar et al. 1994). μCP has a special place in the panoply of direct deposition methods, because it is capable of very high resolu- tion of printing, at a low cost of ownership, thus making it widely used in exploratory research (Delamarche et al. 2003; Delamarche et al. 1997; Kane et al. 1999; Renault et al. 2003). These advantages have led to attempts of applying μCP in many various applications, e.g., patterning neuronal cells (Nicolau et al. 1996; Thiebaud et al. 2002), fundamental stud- ies of cell viability and growth as a function of available space (Amirpour et al. 2001; Chen et al. 1997; Ghosh et al. 2008; Nicolau et al. 1999a), and various microarray and lab-on-a- chip applications (Didar et al. 2012; Hoshino et al. 2014). Protein μCP can be applied to a large variety of substrates such as glass (plain or treated) (Bou Chakra et al. 2008), SAM-coated gold slides (Lee et al. 2008), and polymers, such as polystyrene (Bernard et al. 1998; Bernard et al. 2000).
Although there are several variations of μCP technology (Kaufmann and Ravoo 2010; Kim et al. 2008; Wolfe et al. 2010), all are based on a core process: (i) fabrication of a ‘master ’ , usually made of sil icon using standard microlithography, which presents profiled topographies on its surface; (ii) casting a viscous pre-polymer, usually Poly(dimethylsiloxane), PDMS, on the master; (iii) harden- ing, by curing, of this Brelief stamp^ followed by the detach- ment from the master; (iv) immersion of the stamp in the solution of an ‘ink’, e.g., a solution of a protein; and finally (v) application of the stamp against a flat surface, thus selec- tively transferring the ink from the elevated features to the target surface (Bernard et al. 2000).
Despite these advantages, the central feature of the μCP, i.e., the high compressibility of PDMS, is also the cause of one of important disadvantages: the collapse of the stamp, which leads to deleterious features, e.g., irregular shapes and sizes of the patterns (Huang et al. 2005; Zhou et al. 2005). The present work proposes a design of the master comprising pyramidal wells, which offers a better management of the collapse of the stamp, and better lithographic parameters.
2 Experimental details
2.1 Fabrication of the silicon masters and PDMS stamps
Silicon master The silicon master was fabricated by photoli- thography (spin coating the wafer with positive resist followed by pattern exposure and development), followed by anisotrop- ic etching with a 28%KOH solution along the crystal- lographic face of a silicon wafer, resulting in arrays of pyra- midal wells (Ayeyard et al. 2010). The master comprised a variety of geometries, i.e., three series of arrays arranged in
two rows, each including three arrays of 5 × 5 pyramidal wells. The wells forming the arrays in each row have same size (4 and 8 μm) but increasing inter-well distance (8, 16, 32 μm for 4 μm well size; and 10, 20, 40 μm for 8 μm well size; for detailed design of the silicon master see Supplementary Information – Fig. SI1). The following no- menclature will be used throughout the text; i.e., [number1 μm base]/[number2 μm pitch] representing [the pyramidal base size]/[pitch size between two pyramids]. The wafers were cut into 1 cm × 1 cm chips, each comprising 60 microarrays, and further used as masters for the replication of PDMS stamps.
PDMS stamp The PDMS stamp was fabricated using poly- dimethylsiloxane (PDMS; Sylgard 184, Dow-Corning) fol- lowing a well-known procedure (Duffy et al. 1998) with mi- nor modifications. Briefly, ten parts of pre-polymer were mixed with one part of the cross-linker and degassed under vacuum for one hour. The mixture was then gently poured on top of the silicon master and cured for two hours at 65 °C. The cured polymer was then peeled off from the master and left at 85 °C overnight.
2.2 Protein patterning
Rabbit IgG (2 mg/ml in PBS 10 mM, Molecular Probes), was diluted to 50 μg/mL with PBS 10 mM (0.1 M phosphate buffer, 10 mM NaCl) and adsorbed over a freshly prepared PDMS stamp (100 μL) for 40 min. The stamp was subse- quently rinsed thoroughly with PBS 10 mM (3 × 100 mL) and MilliQ water (3 × 100 mL), air dried and immediately stamped over a cleaned glass coverslip. Conformal contact was allowed to occur spontaneously and stamping was carried out for 60 s, at room temperature, without the use of additional pressure. Subsequently, the IgG-printed substrates have been incubated with a solution of secondary anti-rabbit IgG, Fluorescein labelled (same protocols as above) for 1 h. The fabrication of the Si masters, the PDMS stamps, and the μCP of protein patterns are presented in Scheme 1.
To compare the image quality of the μCP patterns and those obtained by classical microarrays, identical chemicals and solutions, (buffers, protein concentration, fluorophores) and processing conditions (humidity), have been also used to fabricate a microarray using an Inkjet robotic spotting MicroArraying System (PerkinElmer Piezorray) according to methodology described elsewhere (Abdo et al. 2005).
2.3 Imaging and analysis of the masters, stamps and protein patterns
The AFM imaging and analysis was carried out on an Explorer system (Thermo Microscopes) in the normal contact mode, captured by the SPMLab Version 5.01 software.
9 Page 2 of 7 Biomed Microdevices (2016) 18: 9
Images were obtained using an 8 μm Z, linearized scanner (100 μm × 100 μm) under air conditions of temperature o